| ||Format||Pages||Price|| |
|6||$45.00||  ADD TO CART|
|Hardcopy (shipping and handling)||6||$45.00||  ADD TO CART|
Significance and Use
5.1 Moisture in concrete floor slabs affects the performance of flooring systems such as resilient, wood, and textile floor coverings and coatings. Manufacturers of such systems generally require moisture testing be performed before installation of coverings on floor slabs and screeds. The measurement of sub-surface comparative moisture condition in the upper 1.0 in. (25.4 mm) stratum of a concrete slab with a non-destructive moisture meter is one such method.
5.2 Excessive moisture in floor slabs after installation can cause floor covering system failures such as delamination, bonding failure, deterioration of finish flooring and coatings, and microbial growth.
5.3 5.3 Comparative moisture content tests indicate the moisture in the slab, which is usually referenced to the percentage of dry weight. That is:
Results indicate conditions at the time of the test.
5.4 Methods of meter calibration and factors affecting equilibration are described in Section .
1.1 This guide focuses on obtaining the comparative moisture condition within the upper 1.0 in. (25.4 mm) stratum in concrete, gypsum, anhydrite floor slabs and screeds for field tests. Due to the wide variation of material mixtures and additives used in floor slabs and screeds, this methodology may not be appropriate for all applications. See through and Section . Where appropriate or when specified use further testing as outlined in Test Methods , or before installing a resilient floor covering.
1.2 This guide is intended for use to determine if there are moisture-related conditions existing on, or in, the floor slabs that could adversely impact the successful application and performance of resilient flooring products.
1.3 This guide may be used to aid in the diagnosis of failures of installed resilient flooring.
1.4 This guide is intended to be used in conjunction with meter manufacturer’s operation instructions and interpretive data where available.
1.5 Where possible, or when results need to be quantified use this standard guide to determine where additional testing such as Test Methods , , or as specified to characterize the floor slab and the test area environment for moisture, humidity and temperature conditions.
1.6 This guide may not be suitable for areas that have surface applied moisture migration systems, curing compounds or coatings that cannot be removed or cleaned off sufficiently to allow the moisture to move upwards through the slab. For a floor slab of 6 in. (150 mm) plus thickness, low porosity slabs, slabs with no vapor retarder installed, and slabs where the above surface environmental conditions can have a greater than normal influence on the moisture reduction gradient of the floor slab or screed, consider Test Method (below surface in situ rh method) as a more suitable test method under these circumstances.
1.7 This guide is not intended to provide quantitative results as a basis for acceptance of a floor for installation of moisture sensitive flooring finishes systems. Test Methods , , or provide quantitative information for determining if moisture levels are within specific limits. Results from this guide do not provide vital information when evaluating thick slabs, slabs without effective vapor retarders directly under the slab, lightweight aggregate concrete floors, and slabs with curing compound or sealers on the surface.
1.8 The values stated in inch-pound units are to be regarded as standard. The values given in parentheses are mathematical conversions to SI units that are provided for information only and are not considered standard.
1.9 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. Specific warnings are given in Section .
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D4259 Practice for Abrading Concrete
F1869 Test Method for Measuring Moisture Vapor Emission Rate of Concrete Subfloor Using Anhydrous Calcium Chloride
F2170 Test Method for Determining Relative Humidity in Concrete Floor Slabs Using in situ Probes
F2420 Test Method for Determining Relative Humidity on the Surface of Concrete Floor Slabs Using Relative Humidity Probe Measurement and Insulated Hood
ICS Number Code 91.060.30 (Ceilings. Floors. Stairs)
UNSPSC Code 30111500(Concrete and mortars); 30111601(Cement)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM F2659-10(2015), Standard Guide for Preliminary Evaluation of Comparative Moisture Condition of Concrete, Gypsum Cement and Other Floor Slabs and Screeds Using a Non-Destructive Electronic Moisture Meter, ASTM International, West Conshohocken, PA, 2015, www.astm.orgBack to Top